- Nano Express
- Open Access
Study on the CO Oxidation over Ceria-Based Nanocatalysts
© Piumetti et al. 2016
- Received: 8 February 2016
- Accepted: 15 March 2016
- Published: 24 March 2016
A series of ceria nanocatalysts have been prepared to study the structure dependency of the CO oxidation reaction. The ceria samples with well-defined nanostructures (nanocubes/Ce-NC and nanorods/Ce-NR) have been prepared using the hydrothermal method. Mesoporous ceria (Ce-MES) and ceria synthesized with solution combustion technique (Ce-SCS) have also been prepared for comparison. The lowest CO oxidation temperature has been reached by using ceria nanocubes (Ce-NC). This high activity draws immense contributions from the highly reactive (100) and (110) surfaces of the truncated nanocubes. The Ce-MES and Ce-SCS samples, despite their high surface areas, are unable to outdo the activity of Ce-NC and Ce-NR due to the abundant presence of (111) crystalline planes. This finding confirms the structure sensitivity of CO oxidation reaction catalyzed with ceria.
- CO oxidation
- Properties of cerium-based oxides
- Nanostructured ceria
- Ceria-based catalysts
- Structure sensitivity
During the last few decades, ceria-based materials have been widely used for many catalytic applications, including diesel soot combustion, CO oxidation, and VOC abatement [1–4]. These oxidation processes take advantage of the unique redox properties and high oxygen storage capacity (OCS) of ceria. In particular, CO oxidation, a primary function of three-way catalytic converters (TWCs), diesel oxidation catalysts (DOC), and diesel particulate filters (DPF), can be a prototypical reaction for probing the oxidation activity of ceria-based materials [5–8]. As a result, many studies have been carried out to evaluate the catalytic oxidation of CO by ceria and related materials. According to the literature [1, 5, 8, 9], CO oxidation over ceria-based catalysts takes place via a Mars-van Krevelen (MvK)-type mechanism, whereby the reaction involves alternating reduction-oxidation steps on the solid surface with the formation of oxygen vacancies and their successive replenishment by gas-phase oxygen. However, a general consensus has been reached on the fact that CO interaction with ceria is structure sensitive [5, 8]. In addition, it has been revealed that ceria nanoparticles (i.e., nanowires and nanorods), exhibiting an abundance of (110) and (100) crystalline planes, are catalytically more active toward several reactions than CeO2 particles with preferred exposure of stable (111) facets [8, 10–15].
Exposure of specific crystallographic facets, together with the increased number of edges, corners, and facets, is pivotal in controlling the surface reactivity. In fact, nanocatalysts with multifaceted morphologies are highly desirable in catalysis. For fcc metal nanoparticles, the surface energy density (γ) for the three lowest index planes can be ordered as γ (111) < γ (100) < γ (110) [16, 27]. Experimental studies have confirmed that this trend may also hold for ceria-based materials [16, 17]. Theoretical work on the interaction among CO and CeO2 planes have shown the structure sensitivity for CO adsorption, thus suggesting weak CO adsorption for the most stable (111) surface and stronger chemisorption with (100) and (110) facets [18–23]. In this scenario, the metastable ceria (110) surface seems to be the most promising candidate for CO oxidation, since the formation of oxygen vacancies on the (110) planes needs the least amount of energy . Several theoretical studies have shown that the oxygen vacancy formation energy depends on the nature of CeO2 surface [25, 26]. It has also been well-established that the specific surface area of solid catalysts is a key factor in determining their overall catalytic activity in a wide number of catalytic reactions [3, 4, 27]. Therefore, it is necessary to maximize the dispersion of the nanoparticles using high-surface-area supports, such as micro- and mesoporous materials [1, 28, 29].
In the present work, a set of CeO2 samples with different topological and textural properties (CeO2 nanocubes, CeO2 nanorods, mesoporous CeO2, and CeO2 prepared by solution combustion synthesis) has been prepared to investigate the shape-dependency activity of ceria toward CO oxidation, a probe reaction for more complex oxidation processes. Then, the physico-chemical features of the prepared materials have been investigated using complementary techniques.
Synthesis of Samples
CeO2 nanoparticles, denoted further as “Ce-NC” and “Ce-NR” for nanocubes and nanorods, respectively, were prepared via hydrothermal procedure, using sodium hydroxide as the precipitating agent, as we described elsewhere . Mesoporous CeO2, denoted as “Ce-MES,” was synthesized via nanocasting procedure using the SBA-15 silica template . Lastly, a comparative CeO2 sample was prepared via solution combustion synthesis (SCS) and further referred to as “Ce-SCS.” A typical synthesis involved dissolving 3.8 g of Ce(NO3)3·6H2O and 1.8 g of urea in 60 ml of deionized water at room temperature. The homogeneous solution was put into a ceramic crucible and then placed in a furnace at 650 °C for 20 min.
Powder X-ray diffraction (XRD) patterns were acquired on an X’Pert Philips PW3040 diffractometer using Cu Kα radiation. The XRD spectra were recorded in the 2θ range of 20°–70° with 0.02° step size and a time per step of 0.2 s. The diffraction peaks were identified using powder diffraction files by the International Centre of Diffraction Data (ICDD). The average crystallite size was determined using Scherrer’s equation, D = 0.9λ/bcosθ, where λ is the wavelength of the Cu Kα radiation, b is the full width at half maximum (FWHM) in radians, 0.9 is the shape factor for spherical particles, and θ is the angle of diffraction peaks.
BET-specific surface areas (S BET) and total pore volumes (V p) were measured through N2 physisorption at −196 °C on a Micrometrics ASAP 2020 instrument. The samples were previously outgassed at 200 °C for 2 h to remove water and other atmospheric contaminants. The specific surface area of the samples was calculated using the BET method.
Sample morphology was investigated through a field emission scanning electron microscope (FESEM; Zeiss MERLIN, Gemini-II column) and transmission electron microscopy (TEM; Jeol JEM 3010 operating at 200 kV).
Redox properties of the catalysts were investigated by means of X-ray photoelectron spectroscopy (XPS). The measurements were carried out on XPS PHI 5000 Versa probe apparatus using a band-pass energy of 187.85 eV, a 45° takeoff angle, and a 100.0-μm-diameter X-ray spot size. Curve fits were performed by means of Multipack 9.0 software.
Reducibility of the catalysts was determined by H2-TPR measurements. Before the analyses, 50 mg of catalyst was pre-treated under air flow (40 cm3 min−1) at 150 °C for 1 h, to remove water and other atmospheric contaminants, and then cooled to 25 °C with Ar. The analysis was conducted by heating the sample up to 950 °C at a constant rate of 5 °C min−1 under an Ar flow (4.95 % molar H2 in Ar). H2 consumption was recorded using a thermal conductivity detector (TCD).
Catalytic Activity Tests
Catalytic tests for CO oxidation were carried out via a classical temperature-programmed combustion (TPC). The tests were conducted in a fixed-bed quartz reactor (4-mm inner diameter, U-tube) heated by a vertical tubular furnace. The reactor bed comprised of 0.1 g of powder catalyst. A K-type thermocouple was placed at the inlet of the reactor, in such a way that the tip was as close as possible to the catalytic bed. During the reaction, a 50 cm3 min−1 gas containing 1000 ppm of CO and 50 %-vol of air in N2 was continuously fed into the reactor, while the temperature of the furnace increased at a rate of 5 °C min−1 until complete CO conversion was reached. The CO and CO2 concentrations at the outlet of the reactor were measured by NDIR analyzers (ABB Uras 14). Temperatures at which 10, 50, and 90 % of CO was converted were taken as indices of the catalytic activity. The tests were conducted for 2 cycles to evaluate the stability of the catalysts.
Textural and Redox Properties of the Catalysts
Textural properties of the catalysts, as obtained from N2 physisorption at −196 °C and X-ray diffraction analysis 
However, it is worth noting that peak intensities of Ce-MES are rather broad and low. This is most likely due to nanocrystalline ceria frameworks in the sample that constitute mesoporous walls .
Although it is rather difficult to evaluate the average particle size through Scherrer’s formula for morphologies that differ from spherical geometry, an evaluation was conducted to corroborate the TEM results. Scherrer’s equation was employed to estimate the crystallite sizes of the catalysts: Ce-NC, Ce-NR, and Ce-SCS samples possess similar dimensions; the sizes fall in the range of 30–50 nm, whereas the mesostructured sample (Ce-MES) has the smallest particle dimension (5 nm).
The BET surface areas, obtained from N2 physisorption measurement at −196 °C, are very low for both the Ce-NC and Ce-NR samples (4 m2 g−1), thus suggesting a small amount of interparticle voids. In contrast, Ce-MES and Ce-SCS have much higher surface areas than their nanostructured counterparts (75 and 69 m2 g−1, respectively). Indeed, particles in the latter samples are arranged in a network that allows a creation of pores. Ce-MES has higher pore volume than Ce-SCS (0.15 and 0.04 cm3 g−1 for Ce-MES and Ce-SCS, respectively). This supports the fact that pores in Ce-MES are present in mesoscale and that those in Ce-SCS most likely exist in nanoscale.
Results of XPS spectra curve fittings on the O 1s and Ce 3d core level 
Ce3+ (u 1 + v 1) (%-atom)
Reducibility of Catalysts
Catalytic Activity Tests
A series of tests with a classical TPC approach were carried out to investigate the role of structural and electronic properties on the activity of catalysts during CO oxidation reaction. A typical test was conducted according to this sequence: (1) reactor heat-up from ambient to 150 °C with air to remove any possible impurities; (2) introduction of the mixed gas (1000 ppm of CO and 50 %-vol of air in N2) to the reactor; and (3) second reactor heat-up from 150 °C to the temperature at which 100 % CO conversion is reached, (TOS = 2 h at 100 % conversion).
CO oxidation activity results over ceria-based catalysts
In order to evaluate the stability of the catalysts, as well as the reliability of the data, re-tests have been carried out with previously used catalysts. Figure 6b shows CO conversions as a function of temperature over the “used” catalysts. The activity order of the catalysts appears to be preserved, with Ce-NC still being the most active catalyst. Interestingly, it was found that the re-tests with used catalysts resulted in better CO oxidation activity compared to those with “fresh” catalysts. The temperature indicators showed values 10–20 °C lower than those in the tests with fresh catalysts. The exposure of CO during the first cycle might give some carbonate species (e.g., CO3 2−) on the solid surface that would help improve CO oxidation. It is known that oxygen spillover at catalyst surface contributes to the CO oxidation , and so, an abundant presence of surface polycarbonates, stable at high temperature, would have a beneficial effect on the reactivity of ceria nanocatalysts, as already observed by FT-IR analysis over ceria-zirconia catalysts .
As a whole, it has been observed that the catalytic performance for CO oxidation over CeO2 nanocatalysts mainly depends on the presence of highly reactive (100) and (110) surfaces, thus confirming the structure sensitivity for this prototypical reaction. The best results, in terms of CO oxidation, were achieved for the Ce-NC catalyst, due to the abundance of coordinative unsaturated atomic sites in the (100) and (110) exposed surfaces of the CeO2-truncated nanocubes. Moreover, this nanostructured catalyst has shown the lowest reducibility (vide H2-TPR data), thus validating the structure dependency for the CO oxidation reaction. On the other hand, worse CO conversion values were obtained for the high-surface-area catalysts (CeO2-MES and CeO2-SCS), thus showing the key role played by the structural properties of ceria. The least active catalyst was the CeO2-SCS, exhibiting the highest amount of stable (111) planes.
The Ministero dell’Università e della Ricerca (MIUR) (grant number: RBFR12LS6M 001) is acknowledgedfor sponsoring this research activity (FIRB - Futuro in Ricerca 2012). This work was also co-funded througha SINCHEM Grant. SINCHEM is a Joint Doctorate programme selected under the Erasmus Mundus Action 1 Programme (FPA 2013-0037).
Open AccessThis article is distributed under the terms of the Creative Commons Attribution 4.0 International License (http://creativecommons.org/licenses/by/4.0/), which permits unrestricted use, distribution, and reproduction in any medium, provided you give appropriate credit to the original author(s) and the source, provide a link to the Creative Commons license, and indicate if changes were made.
- Trovarelli A, Fornasiero P (2013) Catalysis by ceria and related materials, 2nd edn. Imperial College Press, LondonView ArticleGoogle Scholar
- Heck RM, Farrauto RJ, Gulati ST (2006) Catalytic air pollution control: commercial technology, 3rd edn. Wiley-VCH, Hoboken, New JerseyGoogle Scholar
- Ertl G, Knözinger H, Schüth F, Weitkamp J (2008) Handbook of heterogeneous catalysis, 2nd edn. Weinheim, Wiley-VCHView ArticleGoogle Scholar
- Duprez D, Cavani F (2014) Handbook of advanced methods and processes in oxidation catalysis. Imperial College Press, LondonView ArticleGoogle Scholar
- Wu Z, Li M, Overbury SH (2012) On the structure dependence of CO oxidation over CeO2 nanocrystals with well-defined surface planes. J Catal 285:61–73View ArticleGoogle Scholar
- Russo N, Fino D, Saracco G, Specchia V (2006) Supported gold catalysts for CO oxidation. Catal Today 117:214–219View ArticleGoogle Scholar
- Freund HJ, Meijer G, Scheffler M, Schlögl R, Wolf M (2011) CO oxidation as a prototypical reaction for heterogeneous processes. Angew Chem Int Ed 50:10064–10094View ArticleGoogle Scholar
- Royer S, Duprez D (2011) Catalytic oxidation of carbon monoxide over transition metal oxides. ChemCatChem 3:24–65View ArticleGoogle Scholar
- Aneggi E, Llorca J, Boaro M, Trovarelli A (2005) Surface-structure sensitivity of CO oxidation over polycrystalline ceria powders. J Catal 234:88–95View ArticleGoogle Scholar
- Tana, Zhang M, Li J, Li H, Li Y, Shen W (2009) Morphology-dependent redox and catalytic properties of CeO2 nanostructures: nanowires, nanorods and nanoparticles. Catal Today 148:179–183View ArticleGoogle Scholar
- Liu X, Zhou K, Wang L, Wang B, Li Y (2009) Oxygen vacancy clusters promoting reducibility and activity of ceria nanorods. J Am Chem Soc 131:3140–3141View ArticleGoogle Scholar
- Yan L, Yu R, Chen J, Xing X (2008) Template-free hydrothermal synthesis of CeO2 nano-octahedrons and nanorods: investigation of the morphology evolution. Cryst Growth Des 8:1474–1477View ArticleGoogle Scholar
- Guan Y, Hensen EJM, Liu Y, Zhang H, Feng Z, Li C (2010) Template-free synthesis of sphere, rod and prism morphologies of CeO2 oxidation catalysts. Catal Lett 137:28–34View ArticleGoogle Scholar
- Lin KS, Chowdhury S (2010) Synthesis, characterization, and application of 1-D cerium oxide nanomaterials: a review. Int J Mol Sci 11:3226–3251View ArticleGoogle Scholar
- Han WQ, Wen W, Hanson JC, Teng XW, Marinkovic N, Rodriguez JA (2009) One-dimensional ceria as catalyst for the low-temperature water-gas shift reaction. J Phys Chem C 113:21949–21955View ArticleGoogle Scholar
- Sau TK, Rogach AL (2012) Complex-shaped metal nanoparticles: bottom-up syntheses and applications. Wiley-VCH, WeinheimView ArticleGoogle Scholar
- Wang ZL, Feng X (2003) Polyhedral shapes of CeO2 nanoparticles. J Phys Chem B 107:13563–13566View ArticleGoogle Scholar
- Teng B, Jiang S, Guo X, Yuan J, Luo M (2009) A density functional theory study of CO oxidation on CeO2 (110) surface. Acta Chim Sinica 67:2765–2772Google Scholar
- Nolan M (2009) Molecular adsorption on the doped (110) ceria surface. J Phys Chem C 113:2425–2432View ArticleGoogle Scholar
- Muller C, Paulus B, Hermansson K (2009) Ab initio calculations of CO physisorption on ceria (111). Surf Sci 603:2619–2623View ArticleGoogle Scholar
- Huang M, Fabris S (2008) CO adsorption and oxidation on ceria surfaces from DFT + U calculations. J Phys Chem C 112:8643–8648View ArticleGoogle Scholar
- Scanlon DO, Galea NM, Morgan BJ, Watson GW (2009) Reactivity on the (110) surface of ceria: a GGA + U study of surface reduction and the adsorption of CO and NO2. J Phys Chem C 113:11095–11103View ArticleGoogle Scholar
- Alam MK, Ahmed F, Nakamura K, Suzuki A, Sahnoun R, Tsuboi H, Koyama M, Hatakeyama N, Endou A, Takaba H, Del Carpio CA, Kubo M, Miyamoto A (2009) Study of carbon monoxide oxidation on CeO2 (111) using ultra accelerated quantum chemical molecular dynamics. J Phys Chem C 113:7723–7727View ArticleGoogle Scholar
- Cheng Z, Sherman BJ, Lo CS (2013) Carbon dioxide activation and dissociation on ceria (110): a density functional theory study. J Chem Phys 138:014702View ArticleGoogle Scholar
- Nolan M, Fearon JE, Watson GW (2006) Oxygen vacancy formation and migration in ceria. Solid State Ionics 177:3069–3074View ArticleGoogle Scholar
- Nolan M, Parker SC, Watson GW (2005) The electronic structure of oxygen vacancy defects at the low index surfaces of ceria. Surf Sci 595:223–232View ArticleGoogle Scholar
- Liu Y, Wen C, Guo Y, Lu G, Wang Y (2010) Effects of surface area and oxygen vacancies on ceria in CO oxidation: differences and relationships. J Mol Catal A 316:59–64View ArticleGoogle Scholar
- Cejka J, Corma A, Zones S (2010) Zeolites and catalysis: synthesis, reactions and applications. Wiley-VCH, WeinheimView ArticleGoogle Scholar
- Piumetti M, Bensaid S, Russo N, Fino D (2016) Investigations into nanostructured ceria–zirconia catalysts for soot combustion. Appl Catal B 180:271–282View ArticleGoogle Scholar
- Piumetti M, Bensaid S, Russo N, Fino D (2015) Nanostructured ceria-based catalysts for soot combustion: investigations on the surface sensitivity. Appl Catal B 165:742–751View ArticleGoogle Scholar
- Laha SC, Ryoo R (2003) Synthesis of thermally stable mesoporous cerium oxide with nanocrystalline frameworks using mesoporous silica templates. Chem Commun 17:2138-2139Google Scholar
- Ji P, Zhang J, Chen F, Anpo M (2008) Ordered mesoporous CeO2 synthesized by nanocasting from cubic Ia3d mesoporous MCM-48 silica: formation, characterization and photocatalytic activity. J Phys Chem C 112:17809–17813View ArticleGoogle Scholar
- Kumar PA, Tanwar MD, Bensaid S, Russo N, Fino D (2012) Soot combustion improvement in diesel particulate filters catalyzed with ceria nanofibers. Chem Eng J 207–208:258–266View ArticleGoogle Scholar
- Miceli P, Bensaid S, Russo N, Fino D (2015) Effect of the morphological and surface properties of CeO2-based catalysts on the soot oxidation activity. Chem Eng J 278:190–198View ArticleGoogle Scholar
- Agarwal S, Lefferts L, Mojet BL (2013) Ceria nanocatalysts: shape dependent reactivity and formation of OH. ChemCatChem 5:479–489View ArticleGoogle Scholar
- Yang Z, Woo TK, Baudin M, Hermansson K (2004) Atomic and electronic structure of unreduced and reduced CeO2 surfaces: a first-principles study. J Chem Phys 120:7741–7749View ArticleGoogle Scholar
- Agarwal S, Lefferts L, Mojet BL, Ligthart DAJM, Hensen EJM, Mitchell DRG, Erasmus WJ, Anderson BG, Olivier EJ, Neethling JH, Datye AK (2013) Exposed surfaces on shape‐controlled ceria nanoparticles revealed through AC‐TEM and water–gas shift reactivity. ChemSusChem 6:1898–1906View ArticleGoogle Scholar
- Zhang G, Shen Z, Liu M, Guo C, Sun P, Yuan Z, Li B, Ding D, Chen T (2006) Synthesis and characterization of mesoporous ceria with hierarchical nanoarchitecture controlled by amino acids. J Phys Chem B 110:25782–25790View ArticleGoogle Scholar
- Sinha AK, Suzuki K (2005) Preparation and characterization of novel mesoporous ceria-titania. J Phys Chem B 109:1708–1714View ArticleGoogle Scholar
- Brezesinski T, Erpen C, Iimura K, Smarsly B (2005) Mesostructured crystalline ceria with a bimodal pore system using block copolymers and ionic liquids as rational templates. Chem Mater 17:1683–1690View ArticleGoogle Scholar
- Paier J, Penschke C, Sauer J (2013) Oxygen defects and surface chemistry of ceria: quantum chemical studies compared to experiment. Chem Rev 113:3949–3985View ArticleGoogle Scholar
- Fino D, Bensaid S, Piumetti M, Russo N (2016) A review on the catalytic combustion of soot in diesel particulate filters for automotive applications: from powder catalysts to structured reactors. Appl Catal A 509:75–96View ArticleGoogle Scholar
- Miceli P, Bensaid S, Russo N, Fino D (2014) CeO2-based catalysts with engineered morphologies for soot oxidation to enhance soot-catalyst contact. Nanoscale Res Lett 9:254View ArticleGoogle Scholar
- Bensaid S, Russo N, Fino D (2013) CeO2 catalysts with fibrous morphology for soot oxidation: the importance of the soot-catalyst contact conditions. Catal Today 216:57–63View ArticleGoogle Scholar
- Thomas JM, Thomas WJ (2015) Principles and practice of heterogeneous catalysis (2n Edition). Wiley-VCH Verlag, Weinheim, Germany 113-126Google Scholar
- Piumetti M, Bensaid S, Fino D, Russo N (2016) Ceria-zirconia nanocatalysts for CO oxidation: study on surface properties and reactivity. Appl Catal B http://dx.doi.org/10.1016/j.apcatb.2016.02.023